Q: What is meant by "lost wax" casting, and how is it done?
A: The origins of the lost wax process are shrouded in antiquity, but it
has been used for thousands of years to produce objects in metal which could
not be produced any other way, due to the complexity of their form. It permits
anything that can be modelled in wax to be faithfully transmuted into metal,
and is still used today for certain industrial parts, dental restorations,
fine jewelry, and sculpture.
While wax patterns were originally modelled by hand, and this can still
be done, it is now possible to cast wax into molds as well, so that multiple
copies may be made even though the wax pattern is lost in the process. Modern
synthetic rubbers have been developed which capture very fine detail and
can flex to release undercut areas of a model, greatly reducing the number
of mold parts and the number of parting lines necessary, when compared to
the earlier technique of using wet plaster molds. Waxes can be cast either
solid or hollow, as the wax will coat the inside of a mold after it is filled
and poured out. This process is repeated to build up the desired thickness
of wax. The process is slightly different for jewelry and sculpture; the
smaller quantities involved when making jewelry-sized pieces necessitate
some adaptations to overcome the effects of surface tension, such as wax
injection instead of simple pouring, and the use of a vacuum table or centrifugal
casting machine to force metal into molds.
After it is made and touched-up, the wax model is attached to a "pour-cup",
which is funnel-shaped to channel the metal into the mold from the outside,
using "gates"or "sprues" made from rods of wax , and
a venting system is made the same way to convey air and other gasses out
of the mold when it is filled with hot metal. Once the model is set up with
its gates and vents, it is surrounded with a material that will cover it
smoothly when wet and withstand high temperatures when baked. In some places
an ancient technique involving cow-dung and clay is still used; a very fine
mixture is painted on to capture the detail, then coarser layers are added
to build up a mold that can be handled, baked, and poured into.
A modern variation on this method is called "ceramic shell"; instead
of the cow-dung and clay, a silicaceous slurry is used to cover the model
by dipping and/or pouring. Special dry aggregate is then applied to the
wet pattern, either by hand or by using a "fluidized bed", which
blows the dry particles around in a confined space, covering the wet areas
until no more will adhere. The coated pattern is then left to dry a while
and another layer of wet and dry material is applied. This is repeated,
using coarser aggregate on the outermost layers, until a sufficient thickness
has built up so the mold will hold together through the burn-out and pouring.
The other method commonly used is called "investment" casting.
The pattern is set up in much the same way as for ceramic shell, except
that more venting is necessary due to the decreased porosity of the mold
material, which is made using gypsum plaster (plaster of Paris) as a binder
for sand, silica flour, or another refractory aggregate. There are many
proprietary investment mixtures available, or one may choose to mix one's
own. The dry ingredients are mixed with water and poured into a container
or "flask" surrounding the gated model, which is either waxed
down to a board or attached to a commercially available rubber device which
holds the pattern and flask. Jewelry flasks are generally placed in a vacuum
chamber while this mixure is still fluid, where they are boiled at room
temperature to remove air-bubbles clinging to the models. It is helpful
to de-air the investment mixture before pouring it over the wax models,
in order to reduce boiling-over when vacuuming.
Once the plaster mixture has set hard, the flasks are placed in a kiln,
slowly heated to between 1000 and 1250 degrees F, and held at that temperature
until all wax residues have disappeared. The place where the wax was is
now a void- hence the "lost wax" designation for this process.
The metal is then melted and the molds are filled with liquid bronze or
whatever metal is being used. The flask is then allowed to cool, then the
plaster mold is broken away, revealing the metal part, which faithfully
reproduces every detail of the original wax, plus the gates and vents, which
must be cut off. Silver, gold, aluminum, brass, or bronze may be used interchangably
with this method. Special investment materials and melting equipment are
necessary to deal with the higher temperatures of platinum, iron or stainless
steel, but the process is much the same. Lower-melting metals such as tin,
lead, and zinc may also be cast by this method, but there are other easier
methods of casting them, so it is not often done. A variation on the lost-wax
method is also used for casting objects in glass.
RETURN TO UNITED ARTWORKS HOME PAGE